Electrodeposited pt on three dimensional interconnected graphene as a free standing electrode for fuel cell application
View Online / Journal Homepage Journal of Dynamic Article Links < C Materials Chemistry Cite this: DOI: 10.1039/c2jm16541d www.rsc.org/materials COMMUNICATION Electrodeposited Pt on three-dimensional interconnected graphene as a free-standing electrode for fuel cell application† Thandavarayan Maiyalagan,‡ Xiaochen Dong,‡ Peng Chen* and Xin Wang* Received 12th December 2011, Accepted 30th January 2012Published on 13 February 2012 on http://pubs.rsc.org | doi:10.1039/C2JM16541D DOI: 10.1039/c2jm16541d Downloaded by Nanyang Technological University on 23 February 2012 A three-dimensional interconnected graphene monolith was used Recently, a novel 3D interconnected graphene network has been as an electrode support for pulsed electrochemical deposition of reported,14 which opens up a new promising way for the application platinum (Pt) nanoparticles. Pt nanoparticles with well-deﬁned of graphene based materials. Exhibiting an open-pore honeycomb morphology and small size can be obtained by controlling elec- structure, this 3D graphene has an exceptionally large void volume, trodeposition potential and time. Electrochemical characterization high surface area, high corrosion resistance and high electrical was carried out to examine the electrocatalytic activity of this conductivity. All these properties make it ideal as the electrode monolithic electrode towards methanol oxidation in acidic media. support material for fuel cell applications. Firstly, high corrosion The results show that the carbon material surface and structure resistance of the graphene material can signiﬁcantly reduce the have a strong inﬂuence on the Pt particle size and morphology. support corrosion problem, which has been identiﬁed as one of the main reasons for the quick performance loss of fuel cells.15 Secondly, Compared with the three-dimensional scaffold of carbon ﬁbers, high electrical conductivity is essential for efﬁcient electron conduc- the three-dimensional graphene when used as a free-standing tion through the electrode. Compared to the powder form, the unique electrode support resulted in much improved catalytic activity for monolithic nature can better maintain its conductivity by eliminating methanol oxidation in fuel cells due to its three-dimensionally junction resistance when used as an electrode. Thirdly, the high interconnected seamless porous structure, high surface area and surface area of the 3D graphene allows uniform and high loading of high conductivity. catalysts (here, Pt nanoparticles). Lastly, the interconnected pores may potentially offer low resistance to ﬂuid ﬂow and ensure efﬁcient mass transfer during fuel cell operation. In this work, the free-standing 3D graphene was examined for the 1. Introduction ﬁrst time as an electrode support for methanol oxidation and Graphene, a two-dimensional (2D) nanomaterial with a single sheet compared with the free-standing carbon ﬁber (CF) material16 with of carbon atoms packed in a hexagonal lattice, has recently attracted a similar three-dimensional structure. The present investigation attention due to its fascinating properties, such as high surface area, provides insights and demonstrates potentials of this material for extraordinary conductivity due to high charge carrier mobility and fuel cell applications. The 3D graphene electrode poses two major capacity and excellent mechanical strength.1–4 These unique proper- challenges. The ﬁrst one relates to synthesizing and uniformly depos- ties make graphene a promising material for energy conversion and iting nano-sized Pt electro-catalyst throughout the three-dimensional storage applications.5–9 It is believed that developing macroscopic matrix. The second challenge is the formation of the proton conductor three-dimensional (3D) architecture of graphene will further extend network across the three-dimensional electrode connecting the electro- its abilities towards these applications. There are many reports in the catalytic sites and the proton exchange membrane. To address the ﬁrst literature on graphene powder as a catalyst support for fuel cells.10,11 issue, pulse electrodeposition is adopted which ensures that all the The methods of preparation of the Pt nanoparticles and alloys on the deposited Pt nanoparticles (NPs) are electrically accessible. Further- graphene support have attracted much interest in view of superior more, pulse electrodeposition exhibits several advantages over direct electrocatalytic activity for fuel cell applications.12,13 However, similar current electrodeposition in the control of particle size, uniform to conventional fuel cell electrodes, these materials still suffer from distribution and strong adhesion of the NPs on the substrate.17–19 The insufﬁcient Pt utilization due to the segregation by an insulating second issue of protonic conductivity in the fuel cell electrode could be PTFE binder in the real fuel cell electrode. addressed by employing a hydrophilic Naﬁon electrolyte. Towards that end, deposition of Pt-NPs on the 3D monolithic School of Chemical and Biomedical Engineering, Nanyang Technological graphene architecture is designed and improved activity for methanol University, 62 Nanyang Drive, 639798, Singapore. E-mail: WangXin@ oxidation is reported. The improved activity and stability of the ntu.edu.sg; ChenPeng@ntu.edu.sg; Fax: +(65) 6794 7553; Tel: +(65) electrode were attributed to the unique 3D monolithic architecture 6316 8790 with outstanding conductivity and in the absence of junction resis- † Electronic supplementary information (ESI) available. See DOI: 10.1039/c2jm16541d tance, which leads to efﬁcient electron conduction and mass ‡ Both authors contributed equally to this work. transport. This journal is ª The Royal Society of Chemistry 2012 J. Mater. Chem.
View Online 2. Experimental 2.1 Synthesis of 3D graphene foams The 3D graphene foams with continuous single and few-layer graphenes were synthesized by chemical vapour deposition using nickel foam as the template and ethanol as precursors.14,20 Typically, nickel foams (0.5 mm in thickness, 320 g mÀ2 in areal density) were cut into 2 Â 2 cm and placed in a quartz tube furnace with temper- ature gradually increased to 1000 C under H2 (25 sccm) and Ar (50 sccm) environment. After annealing for 10 min to clean the nickel Fig. 1 (a) Photograph of 3D graphene foam and (b) typical Raman spectra measured at different spots of 3D graphene foam reveal the surface, the ethanol vapour was introduced into the tube by H2/Ar existence of single layer (1L) and few-layer (ML) domains. mixture gas at ambient pressure. 20 min later, the samples were rapidly cooled to room temperature at a rate of $100 C minÀ1. AfterPublished on 13 February 2012 on http://pubs.rsc.org | doi:10.1039/C2JM16541D the growth process, the nickel substrates were etched away with HCl relatively stable, IG/I2D scales linearly with the number of graphene Downloaded by Nanyang Technological University on 23 February 2012 (3 M) solution at 80 C to obtain free-standing 3D graphene foams. layers (up to 4 layers).23 The Raman D-band (at $1350 cmÀ1) is originated from the 2.2 Electrochemical deposition disordered carbon in graphene, and its intensity indicates the density of defects in the as-grown graphene ﬁlm.24 The extremely weak A pulse potential proﬁle of 0 mV (500 ms)À1000 mV (200 ms)–0 mV D-band in the Raman spectra of the free-standing 3D graphene (500 ms) (vs. Ag/AgCl/3 M KCl) with different numbers of pulses was (Fig. 1b) demonstrates the high quality of the obtained graphene. applied for the Pt deposition. After electrodeposition of Pt particles Fig. 2a and b show the morphology of 3D graphene and carbon from the H2PtCl6 solution, the catalyst modiﬁed three-dimensional ﬁber support (carbon paper). The inset in Fig. 2a shows the surface graphene support (Pt/3D-graphene) was washed with de-ionized morphology of 3D graphene at a higher magniﬁcation. SEM analyses water and then dried. reveal that the carbon paper consists of overlapped crossed ﬁbers (Fig. 2b) and the diameter of the ﬁbers is about 5 mm. Controlling the 2.3 Characterization size and dispersion of Pt NPs on 3D graphene is critical for their application in fuel cells. In our study, the Pt NPs with controllable size The thickness and microstructure of the 3D graphene foams were and dispersion are achieved by controlling the pulse deposition in examined by a WITec CRM200 Confocal Raman spectrophotom- aqueous solution. SEM analyses revealed that pulse deposition eter (laser wavelength 488 nm). The morphology of the samples (200 pulses) led to well deﬁned spherical-type Pt particles uniformly was observed by a ﬁeld-emission scanning electron microscope dispersed on the 3D graphene surface, ranging from 10 to 30 nm in size (JEOL-JSM6700-FESEM). X-Ray diffraction (XRD) patterns were (Fig. 2c). Control experiments by the conventional electrodeposition collected with a Bruker D8 Advanced Diffractometer using Cu Ka technique in 1 mM H2PtCl6 + 1 M K2SO4 at À200 mV vs. SCE for radiation. 2.4 Electrochemical measurements The electrochemical properties of the free-standing 3D graphene electrodes were examined using an Autolab Electrochemical Working Station in a three-electrode system in 0.5 M H2SO4 electrolyte at room temperature. Pt gauze was used as the counter electrode, Ag/AgCl as the reference electrode and 3D graphene as the work electrode directly. Stable data were recorded after 20 cycles. The potential range for cyclic voltammetry (CV) measurements was À0.2 to +1.0 V at a scan rate of 50 mV sÀ1. 3. Results and discussion 3.1. Substrate characterization Fig. 1a provides a photograph of the obtained free standing graphene foam which is ﬂexible and black. The monolithic and porous 3D graphene architecture can be clearly observed in Fig. 1a and 2a. The 3D graphene was characterized by Raman spectroscopy, where two characteristic peaks at $1560 cmÀ1 (G-band) and $2700 cmÀ1 (2D-band)21 are evident. As revealed by the integrated intensity ratio of G and 2D bands (IG/I2D) in the Raman spectrum, the 3D graphene exhibits single- Fig. 2 SEM images of the (a) 3D graphene support (b) carbon ﬁber layer and few-layer domains (Fig. 1b).22 Because IG increases support (c) Pt/3 D-GN catalyst and (d) Pt/CF catalyst. Insets in (a) and monotonically with the increasing graphene thickness whereas I2D is (d) are the enlarged pictures. J. Mater. Chem. This journal is ª The Royal Society of Chemistry 2012
View Online 300 seconds were also conducted. Thus conventional electrodeposition To evaluate the electro-catalytic activity of Pt/3D-graphene leads to higher particle sizes of about 100–200 nm (ESI, Fig. S1†). towards methanol electro-oxidation, cyclic voltammograms were TEM images (ESI†, Fig. S2b) also conﬁrm the Pt particles on 3D recorded in a nitrogen purged solution of 0.5 M H2SO4 containing graphene. The uniform and dense distribution of smaller platinum 1 M CH3OH at a scan rate of 50 mV sÀ1 and the current reported particles on the 3D graphene electrode substrate desirably provides was normalized by the Pt active surface area. On the forward abundant catalytic sites. As a result, high electro-catalytic activity was potential sweep (Fig. 4b), the current increased slowly at lower obtained from the modiﬁed 3D graphene electrode. Similar conditions potentials, and then quickly increased at potentials higher than 0.5 of electrodeposition were employed also for the carbon ﬁber electrode. V. These features of the voltammogram, which are similar to those Fig. 2d shows a low-magniﬁcation SEM image of porous carbon of the Pt metal, suggest that the well dispersed Pt NPs on the 3D paper decorated with Pt NPs. A higher magniﬁcation SEM image graphene are electrochemically active.25 The magnitude of the peak (Fig. 2d, inset) indicates that a large number of NPs, with particle sizes current density is directly proportional to the amount of methanol larger than 30 nm, cover the whole surface of the carbon ﬁber. It is also oxidized at the electrode. The peak current density of the forward observed that the dispersion of Pt NPs is more uniform and denser in anodic peaks (If) observed with 3D-graphene is approximatelyPublished on 13 February 2012 on http://pubs.rsc.org | doi:10.1039/C2JM16541D Pt/3D-graphene than in Pt/CF presumably due to the surface ﬂatness 1.6 mA cmÀ2, nearly two times the peak current density of the carbon ﬁber (0.8 mA cmÀ2); this result suggests that 3D-graphene Downloaded by Nanyang Technological University on 23 February 2012 of 3D-graphene compared to a highly curved surface of carbon ﬁber. Therefore, 3D-graphene is proved to be a better catalyst support than plays a critical role in promoting methanol oxidation of Pt NPs. The carbon ﬁber. current density of commercial Pt/C26 catalysts is 1.39 mA cmÀ2 XRD analysis shown in Fig. 3 reveals that the prepared catalysts which is lower than the 3D graphene catalysts. The ratio of the exhibit a typical face-centered cubic (fcc) Pt lattice structure. The Pt/ forward anodic peak current density (If) to the reverse anodic peak 3D-graphene catalyst shows a diffraction peak at $26 , conﬁrming current density (Ib) can be used to describe the tolerance of Pt that the graphitic nature of 3D-graphene is still maintained after the catalysts to CO and other carbonaceous species. The If/Ib ratio for catalyst preparation. In contrast, the XRD pattern of the Pt/CF commercial Pt/C is about 0.80. The reported value of the If/Ib ratio paper exhibits one broad peak centered at $25.6 , indicating the of commercial E-TEK catalyst is $1 (ref. 27–30) and three-dimen- amorphous nature. The average particle sizes of Pt/3D-graphene and sional Pt-on-Pd bimetallic nanodendrites supported on graphene Pt/CF, calculated from the (1 1 1) peak using the Debye–Scherrer nanosheets is 1.25 (ref. 31). In the present study, the carbon ﬁber- equation, are 7.89 and 13.6 nm, respectively. The particle sizes supported Pt NPs have a similar If/Ib ratio as the E-TEK catalyst. observed by SEM are larger than those estimated from XRD, The 3D graphene-supported Pt NPs have a ratio of 2.25, suggesting implying that the agglomerates comprise much smaller particles, that graphene-supported Pt NPs generate a more complete oxida- particularly in the case of carbon ﬁber. tion of methanol to carbon dioxide. Taken together, the highly conductive Pt/3D-graphene electrode with smaller Pt NPs sizes and 3.2. Intrinsic activity of Pt NPs for methanol electro-oxidation better dispersion of NPs exhibits superior intrinsic activity for methanol electro-oxidation. Fig. 4a shows the cyclic voltammogram of both catalytic substrates in Chronoamperometric measurements of Pt/3D-graphene and nitrogen purged 0.5 M H2SO4. Pt/3D-graphene exhibits larger Pt/CF are shown in Fig. 5, which reﬂect the activity and stability double-layer capacitance than Pt/CF, reﬂecting that the electro- of the catalyst to catalyse methanol. Under a given potential of 0.6 V, chemically active surface area of 3D-graphene is signiﬁcantly larger Pt/3D-graphene shows a higher initial current and a slower decay of than that of carbon ﬁber (Fig. 4a). In addition, the electrochemically the peak current with time, suggesting a better catalytic activity and active Pt area, determined by integrating the hydrogen adsorption stability than Pt/CF. area, is found to be 58% higher for Pt/3D-graphene than for Pt/CF. High catalytic efﬁciency for 3D graphene-supported Pt was The larger Pt area in Pt/3D-graphene is ascribed to better dispersion achieved due to the maximization of the three-phase boundary (TPB) of Pt on 3D-graphene, which is conﬁrmed by the SEM analysis. in the electrode by depositing Pt NPs on the outermost surface area of an established porous network. In our method, a free-standing 3D graphene was constructed; Pt NPs were then electro-deposited on the 3D graphene in a liquid solution. Only those sites that are electrolyte accessible and electron accessible can have the deposition of Pt NPs. The advantages of a catalytic electrode made with this 3D graphene include: (1) its unique monolithic network structure offers continuous and multiplexing pathways for electron conduction; (2) Pt NPs are electrodeposited on the most efﬁcient contact zones with guaranteed electronic and electrolytic pathways in the 3D graphene; (3) the open vacancies (pores) mostly in the meso- to macro-size range can be effectively covered by Naﬁon electrolytes, which facilitates the maximization of the three-phase boundary where the electrochemical reaction takes place; (4) the high porosity of 3D graphene also beneﬁts the mass transfer process within the catalyst layer resulting in further improvement for Pt utilization; and (5) the Pt/3D-graphene electrode also showed higher stability and higher conductivity. Combining these advantages, a much improved performance for Fig. 3 XRD patterns of Pt/3 D-GN and Pt/CF catalysts. methanol oxidation is achieved. This journal is ª The Royal Society of Chemistry 2012 J. Mater. Chem.
View OnlinePublished on 13 February 2012 on http://pubs.rsc.org | doi:10.1039/C2JM16541D Fig. 4 (a) Cyclic voltammograms of Pt/3D-graphene and Pt/CF catalysts in H2SO4 (scan rate: 50 mV sÀ1) and (b) in a mixture solution of 0.5 M H2SO4 Downloaded by Nanyang Technological University on 23 February 2012 and 1 M CH3OH (scan rate: 50 mV sÀ1). metals and their alloys for various electro-catalysis applications or electrochemical sensors. Acknowledgements The authors are deeply grateful to the National Research Foundation (Singapore) for the Competitive Research Program (2009 NRF- CRP001-032) and the Ministry of Education (Singapore) for the academic research fund ARC 2/10 (MOE2009-T2-2-024). Notes and references 1 M. D. Stoller, S. Park, Y. Zhu, J. An and R. S. Ruoff, Nano Lett., 2008, 8(10), 3498–3502. 2 Y. X. Xu and G. Q. Shi, J. Mater. Chem., 2011, 21, 3311–3323. 3 C. Mattevi, H. Kim and M. Chhowalla, J. Mater. Chem., 2011, 21, 3324. Fig. 5 Chronoamperometric curves at 0.6 V for 3600 s of (a) Pt/3D- 4 C. Lee, X. Wei, J. W. Kysar and J. Hone, Science, 2008, 321(5887), graphene and (b) Pt/CF electro-catalysts in 0.5 M H2SO4/1 M CH3OH 385–388. solutions at 25 C. 5 Y. Shao, S. Zhang, M. H. Engelhard, G. Li, G. Shao, Y. Wang, J. Liu, I. A. Aksay and Y. Lin, J. Mater. Chem., 2010, 20, 7491–7496. 6 Y. Zhang, T. Mori, L. Niu and J. Ye, Energy Environ. Sci., 2011, 4, 4517–4521. 7 S. Y. Wang, S. P. Jiang and X. Wang, Phys. Chem. Chem. Phys., 2011, 13, 6883–6891. One additional beneﬁt of this 3D graphene is its much lighter 8 J.-J. Shi, G.-H. Yang and J.-J. Zhu, J. Mater. Chem., 2011, 21, 7343– weight compared to the similar sized carbon ﬁber. This could be 7349. advantageous for applications where the system weight is a critical 9 Y. Sun, Q. Wu and G. Shi, Energy Environ. Sci., 2011, 4, 1113–1132. 10 J. Hou, Y. Shao, M. W. Ellis, R. B. Moore and B. Yi, Phys. Chem. parameter. Chem. Phys., 2011, 13, 4083–4094. 11 Y. Hu, H. Zhang, P. Wu, H. Zhang, B. Zhou and C. Cai, Phys. Chem. Chem. Phys., 2011, 13, 15384–15402. Conclusions 12 Y. G. Zhou, J. J. Chen, F. B. Wang, Z. H. Sheng and X. H. Xia, Chem. Commun., 2010, 46, 5951–5953. Platinum nanoparticles deposited on 3D graphene and carbon ﬁber 13 J.-D. Qiu, G.-C. Wang, R.-P. Liang, X.-H. Xia and H.-W. Yu, J. scaffold by the pulse electrodeposition method exhibit different Phys. Chem. C, 2011, 115, 15639–15645. 14 Z. Chen, W. Ren, L. Gao, B. Liu, S. Pei and H.-M. Cheng, Nat. catalytic activity towards methanol oxidation. This difference in Mater., 2011, 10, 424–428. catalytic activity can be attributed to the geometry difference of these 15 X. Wang, W. Z. Li and Y. S. Yan, J. Power Sources, 2006, 158, 154– carbonaceous supports. The enhancement in the Pt/3D-graphene 159. catalyst is attributed to the superior electrical conductivity, large 16 S. Uhm, H. L. Lee, Y. Kwon and J. Lee, Angew. Chem., Int. Ed., 2008, 47, 10163–10166. surface area and efﬁcient mass transport, and dense coating of small 17 H. Kim and B. N. Popov, Electrochem. Solid-State Lett., 2004, 7, platinum nanoparticles. Detailed electrochemical characterization A71–A74. shows the 3D graphene structure as a new kind of supporting 18 H. Kim, N. P. Subramanian and B. N. Popov, J. Power Sources, 2004, 138, 14–24. material with higher catalytic activity and stability for methanol 19 C. Coutanceau, A. F. Rakotondrainib, A. Lima, E. Garnier, e oxidation. The present approach can be readily extended by deco- S. Pronier, J.-M. Lger and C. Lamy, J. Appl. Electrochem., 2004, e rating free-standing 3D graphene with nanoparticles of other noble 34, 61–66. J. Mater. Chem. This journal is ª The Royal Society of Chemistry 2012
View Online 20 X. Dong, W. Fang, C. Y. Su, Y. H. Chen, L. J. Li, W. Huang and 25 D. Pletcher and S. Sotiropoulos, J. Chem. Soc., Faraday Trans., 1994, P. Chen, Carbon, 2011, 49, 3672–3678. 90, 3663–3668. 21 A. C. Ferrari, J. C. Meyer, V. Scardaci, C. Casiraghi, M. Lazzeri, 26 F. Su, J. Zeng, X. Bao, Y. Yu, J. Y. Lee and X. S. Zhao, Chem. F. Mauri, S. Piscanec, D. Jiang, K. S. Novoselov, S. Roth and Mater., 2005, 17, 3960–3967. A. K. Geim, Phys. Rev. Lett., 2006, 97, 187401–187404. 27 V. Raghuveer and A. Manthiram, J. Electrochem. Soc., 2005, 152, 22 Y. Huang, X. Dong, Y. Shi, C. M. Li, L. J. Li and P. Chen, Nanoscale, A1504–A1510. 2010, 2, 1485–1488. 28 T. C. Deivaraj and J. Y. Lee, J. Power Sources, 2005, 142, 43–49. 23 D. Graf, F. Molitor, K. Ensslin, C. Stampfer, A. Jungen, C. Hierold 29 Z. C. Wang, D. D. Zhao, G.-Y. Zhao and H. L. Li, J. Solid State and L. Wirtz, Nano Lett., 2006, 7, 238–242. Electrochem., 2009, 13, 371–376. 24 M. S. Dresselhaus, A. Jorio, M. Hofmann, G. Dresselhaus and 30 S. Guo, S. Dong and E. Wang, Small, 2009, 5, 1869–1876. R. Saito, Nano Lett., 2010, 10, 751–758. 31 S. Guo, S. Dong and E. Wang, ACS Nano, 2010, 4, 547–555.Published on 13 February 2012 on http://pubs.rsc.org | doi:10.1039/C2JM16541D Downloaded by Nanyang Technological University on 23 February 2012 This journal is ª The Royal Society of Chemistry 2012 J. Mater. Chem.